MATERIAL SELECTION OF RF-MEMS SWITCH USED FOR RECONFIGURABLE ANTENNA USING ASHBY’S METHODOLOGY

A. K. Sharma and N. Gupta*

Department of Electrical and Electronics Engineering, Birla Institute of Technology and Science Pilani, Rajasthan 333 031, India

Abstract—This paper reports material selection methodology for radio frequency — micro electro mechanical systems (RF-MEMS) switches used for reconfigurable antennas. As there are variety of materials available to design engineer, a proper technique to select the best possible material is needed. Three primary performance indices, pull-in voltage, RF-loss, and thermal residual stress, are used to obtain the desired performance. The selection chart shows that aluminum is the most suitable material for being used as bridge material in RF-MEMS switches to provide the best performance in reconfigurable antenna.

1. INTRODUCTION

With tremendous advancement in the field of wireless communication, the need for reconfigurable communication devices is always felt. Therefore, the reconfigurable antennas (RA) have received significant attention in recent communication systems because a single RA can be used to change the operating frequency, radiation pattern and directivity based on different application requirements. RF-MEMS switches can be equipped with antenna design to make an antenna reconfigurable by changing its geometrical structure for different resonance frequencies.

MEMS technology has significant impact on communication applications [1, 2]. An RF-MEMS switch utilizes mechanical movement of switch beam to achieve a short or an open circuit in transmission line. Cheng et al. [3] demonstrated RF-MEMS capacitive switch based electrically switchable beam steering antenna by integrating two Quasi-Yagi antenna element with Single Pole Double Throw (SPDT) MEMS

*Received 11 February 2012, Accepted 14 April 2012, Scheduled 20 April 2012*

switch. Cheng et al. [4] described a reconfigurable millimeter-wave lens-array antenna based on dc contact MEMS switches with cantilever design and concluded that MEMS bridge resistance and up-state capacitance have the greatest impact on the frequency response of the antenna. Jung and Lee [5] achieved RF switching for a reconfigurable rectangular spiral antenna with a set of capacitive MEMS switches having low power consumption, high Q and low RF loss, to provide scan-beam capability. These RF-MEMS switches are used to change spiral overall arm length for different directions of beam radiation with low RF loss.

So it is shown that the performance of an antenna depends vastly on RF-MEMS switches which in turn depend on suitable material to be used for the switch. Though several material selection strategies [6–9] have been developed in the past, the methodology for selecting the bridge material used in RF-MEMS switches particularly for reconfigurable antenna has never been proposed. Ashby provides a comprehensive material selection strategy with less computation [10]. So the Ashby approach is used in the work to choose suitable material for RF-MEMS switch.

Through literature review [11–14] it has been observed that the possible materials used for bridge material for fixed-fixed beam capacitive shunt switch are gold, aluminum, platinum, molybdenum, copper, nickel, alumina, and silicon nitride. In this study, the key material indices considered for MEMS capacitive switch are Young’s modulus, electrical resistivity, Poisson’s ratio, thermal expansion coefficient, and thermal conductivity.

The purpose of this paper is to present the results of our study on material selection issue. First, in Section 2, we focus on a brief description of Ashby material selection approach. Section 3 discusses RF-MEMS switch bridge design and performance. Section 4 discusses the performance indices required in Ashby’s approach. Section 5 explains results and discussion, and finally Section 6 concludes our study by giving the conclusion of the paper.

2. ASHBY MATERIAL SELECTION APPROACH

by three parameters: functional requirements, geometrical properties, and material properties. The performance of an element is described by

*P* =*f*[(*F G M*)] (1)

Here *P* describes the performance of the element, and*f* describes the
functions of the functional requirement (*F*), geometrical properties (*G*)
and material properties (*M*), respectively.

*P* =*f*1(*F*)*f*2(*G*)*f*3(*M*) (2)

Here element performance is described by individual functions of *F*,

*G* and *M*. So the optimum subset of material can be identified
by single functional requirement. For *F* and *G*, the performance
can be optimized by optimizing the appropriate material indices.
This optimization is conventionally performed using graphs with axes
corresponding to different material indices or material properties [15].

3. RF-MEMS SWITCH BRIDGE DESIGN AND PERFORMANCE

The most common design of switch is fixed-fixed beam capacitive
shunt switch. This switch beam is suspended at a height of *g* above
the dielectric layer on the transmission line. A suspended
micro-machined bridge structure, with a length*L*, width*w*, thickness*t*, and
an actuation electrode of a length *W* as shown in Figure 1(a), can be
approximately modeled as a fixed-fixed beam with these parameters
as illustrated in Figure 1(b).

The switch operates as a digitally tunable capacitor with two states. When a voltage is applied between a switch beam and the pull-down electrode, an electrostatic force is induced on the beam. The beam over the electrode acts as a parallel plate capacitor. When

*L*

*W*

MEMS Bridge

Electrode

**Substrate** Thin dielectric layer

*L*

*W*
*g*

GND

*t*

(a) (b)

the switch beam is in upstate, the transmission line experiences a small capacitance, and when it is in down state, transmission line experiences a high capacitance [12].

But these switches have their limitations however. By using a proper material in the switch beam, these limitations can be removed, and device performance can be optimized.

4. ASHBY APPROACH TO THE BRIDGE MATERIAL SELECTION

The various material properties, such as Young’s modulus (*E*),
Poisson’s ratio (*ν*), thermal expansion coefficient (*α*), thermal
conductivity (*K*), and electrical resistivity (*ρ*), for MEMS bridge
material have been chosen for Ashby approach. Table 1 shows the
material properties related to the considered materials.

Table 1. Material Properties of the considered materials [17].

Material Young’s Modulus
*E*(GPa)

Poisson’s Ratio (ν)

Electrical
Resistivity*ρ*

(Ω-m)

Aluminum 69 0.33 2*.*90*×*10*−8*

Gold 77 0.42 2*.*35*×*10*−8*

Copper 115 0.33 1*.*72*×*10*−8*

Platinum 171 0.39 10*.*60*×*10*−8*

Nickel 204 0.31 9*.*50*×*10*−8*

Silicon Nitride 304 0.3 *>*1012

Molybdenum 320 0.32 5*.*20*×*10*−8*

Aluminum oxide 380 0.22 *>*1012

Material

Thermal
Conductivity*K*

(W/m-K)

Thermal Expansion
Coefficient*α*
(10*−6* _{(}*◦*_{C)}*−1*_{)}

-Aluminum 222 23.6

-Gold 388 14.2

-Copper 315 17

-Platinum 71 9.1

-Nickel 70 13.3

-Silicon Nitride 29 2.7

-Molybdenum 142 4.9

-Performance Indices: (i) Pull-in voltage

Pull-in voltage is an important parameter for RF-MEMS switches. The mechanical design of MEMS switch consists of two parallel plates. At the time of actuation, the sufficient pull-in voltage is applied between the electrode and MEMS Bridge. This pull-in voltage is given by [16].

*V _{p}* =

r

8*k*

27*ε*0*W w*

*g*3 _{(3)}

Here *k* is spring constant; *ε*0 is permittivity of free space; *W*,*w*, and
*g* are the length of the pull down electrode, width of beam, and gap
between the electrode and beam, respectively.

From Equation (3), it is clear that the pull-in voltage can be reduced in three different ways: first by decreasing the height between the bridge and the electrode, secondly by increasing the area of the bridge and lastly diminishing the bridge structure with low spring constant. Out of these possibilities, the third possibility depends on bridge material parameter, so this is an appropriate way to minimize the pull-in voltage.

Now spring constant depends on Young’s modulus of bridge material, which is given as [16].

*k*= 4*E*

µ

*t*
*L*

¶_{3}

(4)
where *E* is the Young’s modulus, and *t* and *L* are the thickness and
length of the beam, respectively. So from Equations (3) and (4) it is
clear that pull-in voltage is directly proportional to the square root of
the Young’s modulus. So, the first material index (*M I*) related to the
pull-in voltage is

*M I*1 =

*√*

*E* (5)

Spring constant also depends on the thermal residual stress and Poisson’s ratio of the beam material which is given by [13].

*k*= 8*γ*(1*−ν*)(*σ*0*−*∆*σ*)*tw*

*L* (6)

where *γ* is geometric factor; *σ*0 is thermal residual stress at reference

temperature;*ν* is Poisson’s ratio; ∆*σ* is the change in thermal residual
stress. So from Equations (3) and (6) it is clear that the second material
index related to the pull-in voltage is

Now temperature variation results in the change in thermal residual stress of the beam which is given by [13].

∆*σ* =*E*∆*α*∆*T* (8)
where ∆*α*is the difference in thermal expansion coefficient between the
beam and substrate, and ∆*T* is the temperature change of the beam.
Equation (8) shows that thermal residual stress is directly proportional
to the thermal expansion coefficient. From Equations (6) and (8), we
can infer that a higher value of thermal expansion coefficient provides
a lower spring constant. So the third material index related to the
pull-in voltage is

*M I*3 =*α* (9)

Therefore, the first performance indices related to the pull-in voltage is;

*P I*_{1} =*f*(*E, ν, α*) (10)

(ii) RF Loss

Second performance index is related to the RF loss which can be reduced significantly by choosing suitable bridge material having good conductivity. RF power dissipated in the beam is given by [16].

*P _{loss}*=

*I*2

*·R*(11)

where*I* is the current in the switch beam, and*R*is the beam resistance
which is given by [13]

*R*= *βρL*

4*tw* (12)

where *β* is a constant and related to the current crowding into the
membrane, and *ρ* is electrical resistivity of the beam. From the
Equations (11) and (12), we can conclude that power loss in beam
structure is directly proportional to the electrical resistivity of the
bridge material. Therefore, the fourth material index related to the
power loss is

*M I*4 =*ρ* (13)

Therefore, the second performance index related to the RF loss in beam structure is

*P I*_{2}=*f*(*ρ*) (14)

(iii) Thermal residual stress

For large RF signals, the MEMS bridge experiences the temperature change due to self heating which further causes the change in thermal residual stress which is given by [13].

where *P _{loss}* is RF power loss, and

*R*is thermal resistance which is given as [13].

_{T H}*R _{T H}* =

*εL*

4*Ktw* (16)

where *K* is thermal conductivity, and *ε* is non-uniform temperature
distribution. The product of electrical and thermal resistances of the
bridge material (*R* *·RT H*) produces the self heating in the MEMS

bridge. From Equations (16) and (11) we therefore conclude that the fifth material index is;

*M I*5 =*RT HR*=

1

*K* *·ρ* (17)

Therefore, third performance index related to the thermal residual stress in beam structure is

*P I*_{3}=*f*

µ

1

*K* *·ρ*

¶

(18)

5. RESULTS AND DISCUSSION

The optimal performance of MEMS bridge material varies with different performance indices. The material selection graphs are used to select the optimal candidate for MEMS bridge material and also used to identify the trade-offs between the conflicting material indices.

Poisson's Ratio (n)

Thermal Expansion Coefficient (10 ( C) )

-6

o

-1

Figure 2 shows the variation between thermal expansion coefficient
(*α*) and Poisson’s ratio (*ν*) for all possible bridge materials. It is
considered that a material with high values of Poisson’s ratio (*ν*) and
thermal expansion coefficient (*α*) is suitable to minimize the pull-in
voltage. From the plot, it is observed that there is a trade-off between
gold and aluminum. Because gold shows a higher value of *ν* with a
lower value of*α*, but aluminum shows a higher value of*α*with a lower
value of *ν*.

Poisson's Ratio (

ν

)

Young's Modulus (*E*) (GPa)

Figure 3. Poisson’s ratio (*ν*) versus Young’s modulus (*E*) for
considered materials.

Young's Modulus (*E*) (GPa)

Electrical Resistivity (

ρ

) (10

Ω

-m)

-8

Thermal Conductivity (*K*) (W/m-K)

Electrical Resistivity (

ρ

) (10

Ω

-m)

-8

Figure 5. Electrical resistivity (*ρ*) thermal conductivity (*K*) for
considered materials.

Figure 3 shows the plot of Poisson’s ratio (*ν*) versus Young’s
modulus (*E*). From Equations (5) and (7), we can suggest a material
with a low value of Young’s modulus (*E*) and a high value of Poisson’s
ratio (*ν*) reduces the pull-in voltage. From the plot we can conclude
that gold and aluminum are the best materials to reduce the pull-in
voltage.

Figure 4 describes the plot of electrical resistivity (*ρ*) versus
Young’s modulus (*E*) to reduce the RF loss for considered materials.
Here we found that aluminum and gold show the minimum value
of Young’s modulus (*E*) and electrical resistivity (*ρ*) to provide the
minimum RF loss.

Figure 5 shows the plot of electrical resistivity (*ρ*) versus thermal
conductivity (*K*). From the plot we can suggest that gold and copper
followed by aluminum provide the minimum thermal residual stress
for a low value of electrical resistivity (*ρ*) and a high value of thermal
conductivity (*K*) of the bridge material.

6. CONCLUSION

Material selection for RF-MEMS capacitive shunt switch with the help of Ashby approach has been discussed in this paper. Three performance indices based on different material indices to enhance the performance of the MEMS Bridge were optimized. Based on material selection charts, we observed that gold and aluminum are the appropriate materials to be used as bridge material in RF-MEMS switch to obtain the desire properties to give the best performance of the switch in reconfigurable antenna. As gold is very expensive material as compared to aluminum, so if we have to go for mass production of switch, we propose aluminum as the best material to be used as bridge material for RF-MEMS switch.

REFERENCES

1. Cetiner, B. A., G. R. Crusats, L. Jofre, and N. Bıyıklı, “RF MEMS
integrated frequency reconfigurable annular slot antenna,” *IEEE*
*Trans. Antennas Propag.*, Vol. 58, No. 3, 626–632, 2010.

2. Jung, C. W., M. J. Lee, and F. D. Flaviis, “Reconfigurable
dual-band antenna with high frequency ratio (1.6 : 1) using MEMS
switches,”*Electronics Letters*, Vol. 44, No. 2, 76–77, 2008.
3. Cheng, S., P. Rantakari, R. Malmqvist, C. Samuelsson, T.

Vaha-Heikkila, A. Rydberg, and J. Varis, “Switched beam antenna
based on RF MEMS SPDT switch on quartz substrate,” *IEEE*
*Antennas Wireless Propag. Lett.*, Vol. 8, 383–386, 2009.

4. Cheng, C. C., B. Lakshminarayanan, and A. Abbaspour-Tamijani,
“A programmable lens-array antenna with monolithically
inte-grated MEMS switches,” *IEEE Trans. Microw. Theory Tech.*,
Vol. 57, No. 8, 1874–1884, 2009.

5. Jung, C. W. and M. J. Lee, “Reconfigurable scan-beam single-arm
spiral antenna integrated with RF-MEMS switches,”*IEEE Trans.*
*Antennas Propag.*, Vol. 54, No. 2, 455–463, 2006.

6. Srikar, V. T. and S. M. Spearing, “Material selection for
microfabricated electrostatic actuators,” *Sens Actuators A*,
Vol. 102, 279–285, 2003.

7. Rao, R. V., “A material selection model using graph theory and
matrix approach,” *Materials Science and Engineering*, Vol. 431,
248–255, 2006.

8. Roth, R., F. Field, and J. Clark, “Multi-attribute utility analysis,”

9. Guisbiers, G., E. Herth, B. Legrand, N. Rolland, T. Lasri, and L. Buchaillot, “Materials selection procedure for RF-MEMS,”

*Microelectronic Engineering*, Vol. 87, 1792–1795, 2010.

10. Ashby, M. F., *Materials Selection in Mechanical Design*, 2nd
Edition, Butterworth-Heinemann, Oxford, UK, 1999.

11. Puyal, V., D. Dragomirescu, C. Villeneuve, J. Ruan, P. Pons, and
R. Plana, “Frequency scalable model for MEMS capacitive shunt
switches at millimeter-wave frequencies,” *IEEE Trans. Microw.*
*Theory Tech.*, Vol. 57, No. 11, 2824–2833, 2009.

12. Ekkels, P., X. Rottenberg, R. Puers, and H. A. C. Tilmans,
“Evaluation of platinum as a structural thin film material for
RF-MEMS devices,” *J. Micromech. Microeng.*, Vol. 19, 065010–
065018, 2009.

13. Palego, C., J. Deng, Z. Peng, S. Halder, J. C. M. Hwang,
D. I. Forehand, D. Scarbrough, C. L. Goldsmith, I. Johnston,
S. K. Sampath, and A. Datta, “Robustness of RF MEMS
capacitive switches with molybdenum membranes,”*IEEE Trans.*
*Microw. Theory Tech.*, Vol. 57, No. 12, 3262–3269, 2009.

14. Alam, A. H. M. Z., M. R. Islam, S. Khan, N. B. Mohd Sahar, and
N. B. Zamani, “Effects of MEMS material on designing a
multi-band reconfigurable antenna,” *Iranian Journal Of Electrical and*
*Computer Engineering*, Vol. 8, No. 2, 112–118, 2009.

15. Reddy, G. P. and N. Gupta, “Material selection for
microelec-tronic heat sinks: An application of the Ashby approach,”
*Mate-rials and Design*, Vol. 31, 113–117, 2010.

16. Rebeiz, G. M., *RF MEMS: Theory, Design, and Technology*, 3rd
Edition, John Wiley & Sons Inc., New Jersey, 2003.

17. Callister, W. D., *Material Science and Engineering:* *An*
*Introduction*, 7th edition, John Wiley & Sons Inc., New York,
2007.

18. Kingsley, N., D. E. Anagnostou, M. Tentzeris, and J. Papapoly-merou, “RF MEMS sequentially reconfigurable sierpinski antenna on a flexible organic substrate with novel DC-biasing technique,”

*J. Microelectromech. Syst.*, Vol. 16, No. 5, 1185–1192, 2007.
19. Reines, I., B. Pillans, and G. M. Rebeiz, “Thin-film aluminum RF

MEMS switched capacitors with stress tolerance and temperature
stability,” *J. Microelectromech. Syst.*, Vol. 20, No. 1, 193–202,
2011.